synthetic bioabsorbable polymers
Post on 14-Oct-2014
Embed Size (px)
Synthetic Bioabsorbable Polymers for ImplantsC. Mauli Agrawal, Jack E. Parr, and Steve T. Lin, editors
ASTM Stock Number: STP1396
ASTM 100 Barr Harbor Drive PO Box C700 West Conshohocken, PA 19428-2959 Printed in the U. S. A.
Library of Congress Cataloging-in-Publication DataSynthetic bioabsorbable polymers for implants C. Mauli Agrawal, Jack E. Parr, and Steve T. Lin, editors. p. cm.--(STP; 1396) ASTM Stock Number: STP1396. Includes bibliographical references. ISBN 0-8031-2870-3 1. Polymers in medicinc Congresses. 2. Biomedical engineering--Congresses. 3. Biomedial matedals--Congresses. I. Agrawal, C. Mauli (Chandra Mauli) I1. Parr, Jack E. II1. Lin, Steve T., 1947- IV. ASTM special technical publication; 1396. R857.P6 $954 2000 610'.28--dc21 00-040612
Copyright 9 2000 AMERICAN SOCIETY FOR TESTING AND MATERIALS, West Conshohocken, PA. All rights reserved. This material may not be reproduced or copied, in whole or in part, in any printed, mechanical, electronic, film, or other distribution and storage media, without the written consent of the publisher.
Photocopy Rights Authorization to photocopy items for internal, personal, or educational classroom use, or the internal, personal, or educational classroom use of specific clients, is granted by the American Society for Testing and Materials (ASTM) provided that the appropriate fee is paid to the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA 01923; Tel: 978-750-8400; online: http:#www.copyright.com/.
Peer Review PolicyEach paper published in this volume was evaluated by two peer reviewers and at least one editor. The authors addressed all of the reviewers' comments to the satisfaction of both the technical editor(s) and the ASTM Committee on Publications. To make technical information available as quickly as possible, the peer-reviewed papers in this publication were prepared =camera-ready" as submitted by the authors. The quality of the papers in this publication reflects not only the obvious efforts of the authors and the technical editor(s), but also the work of the peer reviewers. In keeping with long-standing publication practices, ASTM maintains the anonymity of the peer reviewers. The ASTM Committee on Publications acknowledges with appreciation their dedication and contribution to time and effort on behalf of ASTM.
Printedin Scranton,PA July 2000
ForewordThis publication, Synthetic Bioabsorbable Polymersfor Implants, contains papers presented at the symposium of the same name held in Kansas City, Missouri, on 16-17 November 1999. The symposium was sponsored by ASTM Committee F4 on Medical and Surgical Materials and Devices. The symposium co-chairmen were C. Mauli Agrawal, The University of Texas Health Science Center, Jack E. Parr, Wright Medical Technology, Inc., and Steve T. Lin, Exactech, Inc.
ContentsOverviewMechanical Evaluation of 70:30 Poly (L/DL-Lactide) Bone Screws After In Vitro Degradation--J. A. DISEGI,J. W. DWYER,ANDR. E. FAIRER Evaluation of Adhesive and Absorption Properties for Absorbable TissueA d h e s i v e s - - - J . M. ALLAN, J. A. FLALE, J. D. KLINE, R. L. DOOLEY, AND S. W. SHALABY
Bacterial Polyesters for Biomedical Applications: In vitro and in vivo Assessmentsof Sterilization, Degradation Rate and Biocompatihility of Poly ([3-gydroxyoctaanoate) (PHO)--Y. MAROIS, Z. ZHANG, M.R. W. LENZ, AND R. GUIDOIN VERT, X. DENG,
Novel Biodegradable Polyurethanes for Medical Applications---K. GORNA AND s. GOGOLEWSra Effects of Thermal History and Physical Aging on Thermal Properties of Poly-L-Lactide.---M. DENG,J. M. ALLAN,J. T. CORBETI',AND S. W. SHALABY Resorption Profile and Biological Response of Calcium Phosphate filled PLLA and PI-IB7V--N. L. JONES,J. J. COOPER,R. D. WATERS,ANDD. F. WILLIAMS The Clinical Evaluation of a Bioresorbable Minipin--D. w. HUTMACHER,A. KIRSCH,K. L. ACKERMANN, H. LIEDTKE, AND M. B. HL~RZELER
The Use of the Vibrating Particle Technique to Fabricate Highly Porous And Permeable Biodegradable Scaffolds---c. M. AGRAWAL, J. S. MCKINNEY,D. HUANG, AND K. A. ATHANASIOU
Modulation of Pore Topography of Tissue Engineering Constructs---K. J. L. BURG,C. E. AUSTIN, AND J. P. SWlGGETT
In Vitro Compression Testing of Fiber-Reinforced, Bioabsorbable, Porous Implants--M. A. SLIVKA,N. C. LEATHERBURY, KIESWETTER,AND G. G. NIEDERAUER K. Clinical Evaluation of a Bioresorbable Membrane for Hard Tissue Regeneratiow-D. W. HUTMACHER, A. KIRSCH, K. L. ACKERMANN, AND M. B. HORZELER
Design and Fabrication of a 3D Scaffold for Tissue Engineering B o n e - D. W. HUTMACHER, S. H. TEOH, 1. ZEIN, K. W. NG, J. T. SCHANTZ, AND J. C. LEAHY
Over the past decade, the use of synthetic bioabsorbable polymers in the field of medicine has grown steadily, and it is not uncommon today to find bioabsorbable devices commercially available for use as implants. The popularity of bioabsorbable polymers in medicine stems from the fact that implants fabricated from these materials are absorbed by the body over time. Moreover, the rate of absorption can be designed to meet the needs of the application. This is a significant advantage because nonabsorbable implants often have to be removed surgically after tissue healing has occurred. Also, most synthetic bioabsorbable polymers can easily be injection molded or extruded into a variety of shapes, which facilitates manufacturing and reduces cost. As the awareness and the concomitant use of bioabsorbable devices increases, there is a need to address issues of novel and new applications, test and characterization techniques for raw materials and devices, efficacy, and long-term effects. The purpose of this symposium was to explore these issues, teach the latest developments in applications and test techniques, and promote the standardization of minimum requirements and test methodologies. The papers included in this volume covered a variety of topics such as basic polymer properties and characterization, testing techniques, and tissue engineering. At the present time one of the most popular strategies used in tissue engineering is the implantation of a porous biodegradable scaffold at the defect site in the tissue. This scaffold may carry cells or other biomolecular signals to enable tissue regeneration. Synthetic biodegradable polymers are often used for the scaffolds, and thus, play an important role in tissue engineering. Also discussed were various aspects of biodegradable scaffolds. Lastly, bioabsorbable polymers are receiving attention as replacements for metallic fracture fixation devices and systems. This STP provides an overview of the use of synthetic bioabsorbable polymers in the medical field at the present time. We predict that in the future such materials will play a very significant role as implants. We would like to thank the ASTM staff (Dorothy Fitzpatrick, Teresa Cendrowska, and Annette Adams) for working so diligently on this project.
C. Mauli AgrawalThe Universityof Texas Health ScienceCenter San Antonio,Texas SymposiumChairmanand Editor
Jack ParrWright Medical Technology,Inc. Arlington,Tennessee SymposiumChairmanand Editor
Steve LinExactech Gainesville,Florida SymposiumChairmanand Editor
John A. Disegi, l James W. Dwyer, I and Robert E. FairerIMechanical Evaluation Of 70:30 Poly (L/DL-Lactide) Bone Screws After In Vitro Degradation
Reference: Disegi, J. A., Dwyer, J. W., and Fairer, R. E., "Mechanical Evaluation of 70:30 Poly (L/DL-Lactide) Bone Screws After In Vitro Degradation," Synthetic Bioabsorbable Polymersfor Implants, ASTMSTP 1396, C. M. Agrawal, J. E. Parr, and S. T. Lin, Eds., American Society for Testing and Materials, West Conshohocken, PA, 2000. Abstract: Controlled in vitro degradation testing is typically used to complement animal trials in order to understand the material, design, and fabrication factors that affect in vivo resorption rates of bioabsorbable implants. Resorbable 1,5 mm craniofacial bone screws were injection molded from amorphous 70:30 poly (L/DL-lactide) granules. The screws were vacuum dried, bulk packed, and gamma sterilized. Some of the screws Were fully immersed in 7.4 pH phosphate buffer solution. The solutions were maintained at 37~ during short term exposure periods that extended to 8 weeks. Non-exposed control samples were stored in sterilized packages until the testing commenqed. Stability testing was performed with rigid polyurethane foam to evaluate whether this test material was satisfactory for use in phosphate buffer solution. Screw pull-out strength was measured in accordance with ASTM. F 1691. Shear strength before and after in vitro degradation was analyzed by determining the maximum applied force required to shear the screw shaft when mounted in a specialized test fixture.
Keywords: degradation-surgical devices/applications, poly(L-lactic acid), testing methods-surgical implants, pull-out fixation strength, shear testing-medical materials/applications
Maxillofacial plates and screws produced from resorbable polymers have been evaluated by a number of researchers. The use of resorbable materials represents an ideal fracture fixation application since these implants are small in mass and subjected to relatively low stress during implantation. Initial fracture stabilization !s extremely important because critical fracture healing of highly vascularized craniofacial regions may occur within a four to six week implantation period. Controlled in vitro degradation testing is commonly used to complement animal trials in order to understand the material, design, and fabrication factors that affect in vivo resorption rates. The present study rMaterials development manager, product development engineer, and mechanic